Viscoelastic Properties of Fresh Cement Paste to Study the Flow
, Kyoungsoo Park2)
, and Taekeun Oh3),
(Received March 23, 2016, Accepted June 6, 2016, Published online June 28, 2016)
Abstract: During concrete pumping, the migration and redistribution of particles occur in a pipe and the lubrication layer that forms between the bulk concrete and the pipe wall is the governing factor determining the ﬂow behavior. In order to identify ﬂow behavior of pumping, in this study, the viscoelastic properties related to the microstructural behavior of a ﬂocculated suspension were examined by using dynamic oscillatory measurements. Cement paste is assumed to be a constituent material of the lubrication layer and ten cases of mixing design are employed by changing the proportions of mineral admixtures. The relationship between the yield stress obtained from the steady shear test and the dynamic modulus resulted from the oscillatory shear measurement was derived and the implications of the correlation are discussed. Moreover, based on the investigation of the viscoelastic properties with oscillatory measurements, the initial behavior of pumped concrete was analyzed systematically.
Keywords:concrete pumping, lubrication layer, dynamic oscillatory measurement, viscoelastic.
Concrete pumping involves the ﬂow of a complex ﬂuid under high pressure in a pipe, and thus predicting ﬂow behaviors of concrete pumping is challenging research area. For the characterization and prediction of the ﬂow of con-crete pumping, the fundamental understanding of various factors is needed, which include rheological properties, dynamic segregation, stability of constituent materials, geometry of a pumping circuit, slip layer formed between bulk concrete and a pipe wall, and relationship between the pressure and ﬂow rate. The ﬂow of concrete in a pipe differs from the one of typical viscous ﬂuids like water or oil. The primary difference is that concrete is a yield stress ﬂuid. Therefore, there is at the center of the pipe (i.e. around the symmetry axis where the shear stress is equal to zero) a zone where the concrete is not sheared (Jacobsen et al. 2009). Most researches on concrete pumping in the literature account for the yield stress and the existence of the unsheared zone (Vassiliev 1953; Kaplan et al. 2005; Feys
and Schutter 2005) by assuming that concrete behaves as either the Bingham ﬂuid or the Herschel Buckley ﬂuid. The second reason for the difference is that under the action of shear, the redistribution of particles occurs within a pipe, which is a common feature of particle suspensions. Initially well mixed particles in a concentrated suspension ﬂows undergo migration from high shear rate regions to low shear rate regions (Phillips et al.1992; Ingber et al.2009; Lu et al. 2008). During concrete pumping, shear concentrates in the ﬂuid layer of material depleted of the coarsest particles of concrete. Therefore, the pumping of concrete can be gener-ally considered to be the shearing of an annular layer of unknown thickness and made of a material with certain rheological properties.
While particle collisions in highly sheared and/or highly concentrated zones enforce particles to migrate from these zones, it is counterbalanced by the local increase in concrete viscosity resulting from this migration (i.e. in the bulk). The shear induced particle migration (Choi et al.2013a) is due to the competition between gradients in particle collision fre-quency and gradients in the viscosity of concrete within a pipe. When cement particles migrate, they encounter a high viscosity of bulk concrete, in which sand and gravel particles have already migrated and should be prevented from migrating inside the bulk. Therefore, the migration of small particles like cement particles can be neglected, compared to the migration of large particles, such as sand and gravel particles. Because of such migration characteristics, the slip layer is generated along the high shear and/or concentrated zone, which can be considered, as an approximation, as being similar to the constitutive cement paste in concrete pumping. This layer is often called the lubrication layer or the slippage layer.
1)Department of Safety Engineering, Dongguk
University-Gyeongju, Gyeongju, Korea.
Department of Civil and Environmental Engineering, Yonsei University, Seoul, Korea.
Department of Safety Engineering, Incheon National University, Incheon, Korea.
*Corresponding Author; E-mail: firstname.lastname@example.org
CopyrightÓThe Author(s) 2016. This article is published with open access at Springerlink.com
International Journal of Concrete Structures and Materials Volume 10, Number 3 Supplement, pp.S65–S74, September 2016 DOI 10.1007/s40069-016-0158-3
The existence of the lubrication layer was ﬁrst suggested by Aleekseev (1952) and Weber (1968). Morinaga (1973) noted that based on theoretical ﬂow behaviors of concrete, the pumping of concrete would not be possible without the formation of the lubrication layer. Sakuta et al. (1979) reported that the ﬂow properties of the bulk material were irrelevant; the only property that matters is the ability of the material to form this layer. Jacobsen et al. (2009) conducted experimental research with colored fresh concrete after ﬂowing ordinary concrete to observe the ﬂow conditions in various pipes. Rossig and Frischbeton (1974) pumped col-ored concretes in a pipe for the direct observation of the ﬂow proﬁles. Their results revealed the existence of a high velocity and paste rich zone at the vicinity of the pipe wall. The thickness of the lubrication layer was estimated in the range of 1 mm and 5 mm (Choi et al.2013a,b; Browne and Bamforth1977). Feys and Schutter (2005) reported that the thickness and rheological properties of the layer appear to depend on the mix proportions of the pumped concrete. The macroscopic consequences of this layer on the pumping pressure were considered by introducing interface properties measured macroscopically using a tribometer to the pumping process prediction (Kaplan et al. 2005). In summary, the formation and characteristics of the lubrication layer are essential on concrete pumping and thus a detailed analysis of the layer is necessary to understand ﬂow behaviors.
Several studies have examined the rheology of cement slurries which is the constituent material of the lubrication layer for other applications, which include the descriptions of the thixotropic behavior (Papo 1988), and the hysteresis effects in the shear rate/shear stress relationship (Xuequan and Roy 1984; Atzeni et al. 1985; Grzeszczyk and Kucharska 1988). Modiﬁed consistometers have been applied to provide gel build up information, as used by Keating and Hannant (1990). Banﬁll and Kitching (1990) used controlled stress rheometers to examine the yield stresses of cement slurry.
As one of the important information of the rheology, the viscoelastic properties are associated with the slurry microstructure. Several researchers have investigated vis-coelastic properties of cement slurry mixtures. Tattersall and Banﬁll (1983) demonstrated that the paste undergoes the breakdown of structure while the amplitude of shear increases. Cooke et al. (1988) examined viscoelastic parameters for both ﬂowing and curing cement slurries. Chow et al. (1988) discussed the use of the viscoelastic parameters as an alternative to consistometer studies. Saaka et al. (2001) measured viscoelastic properties of cement paste, and illustrated the effect of wall slip on the shear yield stress. Figura and Prud’homme (2010) considered the vis-coelastic response of cements with curing-rate control additives. However, little attention has been paid to the viscoelastic properties of ﬂowing materials for examining the ﬂow behaviors, particularly in the pumping industry.
Therefore, the present study examined the viscoelastic properties using dynamic oscillatory measurements to quantify the ﬂow behavior of concrete pumping. Dynamic modulus measurements on the cement paste, which could be
considered a constituent material of the lubrication layer, were taken. Steady shear measurements were simply con-ducted to examine the basic rheological properties like the yield stress and the plastic viscosity while the dynamic oscillatory tests were performed to evaluate the dynamic modulus. The relationship between the measured yield stresses and the dynamic modulus was derived and the implications of the correlation are discussed.
2. Theoretical Background for Viscoelastic
A dynamic oscillatory shear test is a rheological technique that provides information on viscoelastic materials. This is a dynamic method, in which strain or stress oscillates according to a sinusoidal function. The measured output is the level of stress or strain and the extent to which the stress and strain is in phase with the applied strain or stress. By limiting the strain to small amplitude, the particles remain in close contact with one another and the microstructure is not disturbed.
When a material of a yield stress ﬂuid is sheared under an applied sinusoidal oscillation with a sufﬁciently small amplitude, the measured dynamic behavior may be linear and can be analyzed in terms of the theory of linear vis-coelasticity. Details of the theory and the methods for measuring the viscoelastic properties are well documented in the literature (Ferry1970; Marin1988; Nguyen and Boger 1992; Schultz and Struble1993).
In general, the oscillatory strain at time tis deﬁned as
wherecis the strain at timet,c0is the strain amplitude, and xis the frequency. The resulting shear stress is sinusoidal and proportional to the shear strain in the out-of-phase mode
where s0 is the maximum shear stress and d is the phase angle between the applied strain wave and the stress response. The shear stress (Eq. (2)) can be expressed using two viscoelastic terms, in-phase term and out-of-phase term, as expressed below;
s¼s0þs00¼c0ðG0sinðxtÞ þG00cosðxtÞÞ ð3Þ
effect and the viscous effect. Through the dynamic oscilla-tory measurements, the oscillaoscilla-tory parameters, G0 and G00, can be analyzed to determine viscoelastic properties.
3. Experimental Program
The redistribution of particles under the action of shear occurs within a pipe and the lubrication layer can be con-sidered as being similar to the constitutive cement paste of pumped concrete, as discussed in Sect.1. Based on this assumption, the material for the lubrication layer was obtained from wet-screened cement paste from fresh con-crete. The compressive strength of 50 MPa was selected, as shown in Table1. Portland cement CEM I 52.5N was used with the speciﬁc gravity of 3150 kg/m3. Three types of mineral admixtures were selected, i.e. blast furnace slag (BFS) with the speciﬁc surface area of 3950 cm2/g, ﬂy ash (FA) with 3060 cm2/g, and silica fume (SF) with 200,000 cm2/g. Table2 lists the chemical compositions of the cement and mineral admixtures. The concrete mixes were designed as unitary, and binary blends by replacing cement with mineral admixtures in the study, as shown in Table3. The sand was natural river sand with the density of 2590 kg/m3 and ﬁneness modulus of 2.81. The sand parti-cles ranged in size from 0.08 to 5 mm with the water absorption capacity of 2.43 %. The coarse aggregate was limestone with the water absorption capacity of 0.8 %, the density of 2610 kg/m3, and the ﬁneness modulus of 6.72. The maximum coarse aggregate size was 20 mm. The amount of mixing water was corrected to consider the water absorbed by the ﬁne and coarse aggregates. A polycar-boxylate-based high-range water-reducing admixture (HRWRA), which is marked as % HRWRA, meaning the percentage of the admixture relative to the binder content (in weight) was used to obtain the target slump ﬂow.
3.2 Test Procedure
A rheometer was used to measure the rheological prop-erties. In addition to the steady shear measurements, the rheometer is also capable of continuous strain sweep (i.e., at a constant frequency of oscillation the amplitude of the
displacement is continuously varied) and frequency sweep (i.e., at a constant stress or strain of oscillatory measure-ments the frequency of the oscillation is continuously var-ied). In this study, a parallel plate geometry was adopted to minimize the effects of the particle settling of particles during the measurements. The radius of the bob plate was 25 mm and the distance between the two parallel plates was 1.5 mm. The surface of the bob plate was serrated, as pro-vided by the manufacturer to avoid slippage during the measurement (Fig.1). The temperature of the rheometer was 25°C.
Two different measurement procedures were employed, i.e. steady shear and dynamic oscillatory shear. For the steady shear measurement, the sample was subjected to a stepped ramp with 20 different shear rates starting from 0.1 to 550 s-1after a 275 s-1continuous shear for 30 s. Sub-sequently, the data were acquired at a descending shear rate from 550 to 0.1 s-1 with 20 steps, allowing 10 s at each step. Figure2 presents a schematic representation of the steady shear program. Three replicate tests are performed for each case of mixing design.
For the dynamic oscillatory measurement, it is important to use a strain within the linear viscoelastic region (LVR). To ensure that the measurements were in the LVR, the strain and frequency sweeps were initially performed and checked to identify the LVR. These experiments conﬁrmed that the measurements with the 0.1 % strain and the 1 rad/s fre-quency resulted in the LVR over the course of the experi-ment. Thus, strain sweeps were performed at a constant frequency of 1 rad/s within the LVR, ranging from 0.001 to 10 % strain. Frequency sweeps were performed at a constant strain amplitude of 0.1 % within the LVR ranging from 0.01 to 100 rad/s.
4. Results and Discussions
4.1 Steady Shear Properties
Figure3shows the relationship between the shear rate and the shear stress from the steady shear measurement for the mixtures. The Bingham model was used to determine the yield stress, sy, and the plastic viscosity, l. Most of the cement slurry data followed this Bingham model quite well;
Table 1 Mixture proportions for C50 (Unitary).
Design strength C50
Cement (kg/m3) 500
Sand (kg/m3) 736
Coarse aggregate (kg/m3) 871
% Polycarboxylate-based HRWRA* 0.9
Slump ﬂow (mm) 600±20
the viscosity was relatively linear over the range of shear rates. Table4 lists the calculated Bingham parameters obtained from ﬁtting the data in Fig.3. The measurements indicated the following:
1. The plastic viscosity and the yield stress of the constitutive cement paste are varied according to the types and replacement ratios of the mineral admixtures. Table 2 Chemical compositions of raw materials used in the study (wt%).
Chemical compositions OPC BFS FA SF
Al2O3 4.19 14.55 23.66 1.30
SiO2 17.76 29.98 49.83 92.00
Fe2O3 3.24 0.50 9.03 2.40
CaO 67.16 45.92 8.77 –
MgO 2.26 4.90 1.83 0.40
TiO2 0.23 0.73 1.62 –
K2O 1.21 0.60 1.97 1.20
Na2O 0.09 0,21 0.72 0.10
SO3 2.99 – 0.96 –
Loss on ignition 0.84 – 2.88 –
OPCordinary portland cement,BFSblast furnace slag,FAﬂy ash,SFsilica fume.
Table 3 Mix designs.
Blended types Notation W/B OPC (%) Mineral admixtures (%) HRWRA (%)
BFS FA SF
Unitary UO 0.33 100 – – – 0.9
Binary BFS40 60 40 – –
BFS50 50 50 – –
BFS60 40 60 – –
FA10 90 – 10 –
FA20 80 – 20 –
FA30 70 – 30 –
SF5 95 – – 5
SF10 90 – – 10
SF20 80 – – 20
Fig. 1 Serrated bob plate used in the measurements to minimize the effects of slip and settling.
Fig. 3 Results of steady shear measurement.aAll cases,bUO and BSF cases,cUO and FA cases,dUO and SF cases.
Table 4 Rheological parameters calculated from the steady shear measurements and the dynamic oscillatory measurements.
Blended types Notation Steady shear measure Dynamic oscillatory
sy (Pa) l(Pa s) G
Unitary UO 13.6 0.134 1.49E?02
Binary BFS40 10.6 0.132 6.43E?01
BFS50 9.3 0.106 6.19E?01
BFS60 9.0 0.055 3.51E?01
FA10 15.1 0.058 1.62E?02
FA20 20.3 0.097 1.65E?02
FA30 24.3 0.132 6.78E?02
SF5 3.5 0.123 8.90E?00
SF10 25.7 0.069 6.90E?02
2. When the replacement ratio of BFS increases, the yield stress and the plastic viscosity of the constitutive cement paste gradually decrease in this study. The measured rheological properties of the mixes with BFS are lower than the mix without BFS, which indicates that BFS improves ﬂowability in this system. This is because the BFS particles ﬁll into spaces among larger particles and decrease frictional forces of matrix.
3. The yield stress and the plastic viscosity slightly increase when the replacement ratio of FA increases. The FA, from a theoretical point of view, should improve ﬂowability as the spherical shape of FA reduces the frictional force among the angular parti-cles, as called ball bearing effect. However, there is a critical factor making worse ﬂowability. The unburned carbon in FA is known to adsorb superplasticizer (SP), which lead to worse workability of matrix. Therefore, in case of the FA mixes tested, the effects of unburned carbon are a more governing factor than the ball bearing effect.
4. The yield stress and plastic viscosity of SF mixtures decrease at 5 % replacement but increase steeply as the SF reaches more than 10 % replacement. Based on these rheological test results for the SF mixes, the ball bearing effect due to the spherical shape of SF could be governing the ﬂowability of matrix at 5 % replacement. However, when the replacement of SF is greater than 5 %, e.g. 10 and 20 % replacement, because of the high speciﬁc surface area of the very ﬁne particles of SF (mean size&0.1lm), the SF particles become highly reactive and easily adsorb SP molecules, which form multi-layers. As the replace-ments with SF exceed 5 %, the quantity of SP in the system decreases substantially because the signiﬁcant adsorption of SP into the SF occurred, which leads to a steep increase in the yield stress and plastic viscosity at 10 and 20 % replacements.
4.2 Viscoelastic Properties
Figure4 presents one of test results of a dynamic oscil-latory shear using strain sweep and frequency sweep. Based on the measured test results, the storage modulus, G0 (rep-resenting the elastic portion in viscoelastic materials), and the loss modulus,G00(representing the viscous portion). The strain sweep showed variations in the storage modulus with strain amplitude, which was expected for a ﬂocculated sus-pension. The storage modulus, G0, was independent of the strain up to 0.3 % strain amplitude and then at higher strain amplitude, the storage modulus decreased with increasing strain amplitude. This reﬂects the breakdown of the ﬂoccu-lated network structure as the strain is increased. The product of the modulus and the strain at which breakdown is ﬁrst observed, i.e. the ‘‘critical strain’’ cc, is the threshold for breakdown and has been associated with the yield stress of the system under static conditions. This static yield stress is not necessarily related to the yield stress under ﬂowing conditions, which is reﬂected in the Bingham or Herschel-Bulkley yield stresses. The loss modulus, G00, was smaller than the storage modulus at LVR, indicating a solid-like response, where most of the stress in the system is supported by the solid colloidal network structure. As the strain amplitude goes beyond the critical value, the loss modulus becomes higher than the storage modulus, which means the behavior changes to a more ﬂuid-like response. Note that the level ofG0 is still signiﬁcant, and this structure results in a yield stress in steady ﬂow.
Based on the results of the strain sweep, the strain amplitude of 0.1 %, which exists completely within LVR, was selected for the frequency sweep measurement ranging from 0.01 to 100 rad/s. In Fig.4b, the frequency sweep showed a plateau inG0in the applied frequency region, over which the modulus varied slightly with frequency. The fre-quency applied for the strain sweep test, 1 rad/s, also lays on this plateau. As in the strain sweep, the storage modulus in the frequency sweep was higher than the loss modulus in the
region tested. Both parameters for the dynamic oscillatory tests were within the LVR and the frequency sweep tests were then performed. The results are shown in Fig.5. The observations for the storage modulus, G0, complement the observations from the steady shear ﬂow results. Several conclusions can be drawn from these measurements:
(1) The dispersions were all structured and displayed G0 values that were essentially unchanged over the experimental frequency range.
(2) The storage modulus in the frequency sweep decreased gradually in the region tested as the replacement ratios of BFS were increasing but the difference between BSF40 and BSF50 was not distinguished clearly. In the case of FA mixtures, the storage modulus increased slightly with increasing replacement ratios of FA but this was not observed clearly. On the other hand, the SF mixtures showed a clear difference. The storage modulus decreased at 5 % replacement but increased steeply when the SF was over 10 % replacement. The overall variation of the oscillatory shear measurement has a close relationship with the results of the steady shear measurement.
(3) A comparison with the results of the steady shear measurement showed that the tendency of the calcu-lated yield stress follows the trend of the storage modulus variation. Therefore, in this study, a detailed investigation was conducted to determine the relation-ship between the variation of the storage modulus and yield stress.
4.3 Relation Between the Yield Stress
and the Dynamic Moduli
The yield stress provides information concerning the microstructure of the sheared suspension. In this experiment, it is the structure that exists as the shear rate is decreased. In dynamic oscillatory shear, the storage modulus and critical strain are related to the fundamental microstructural aspects of the ﬂocculated suspension at rest (Schultz and Struble 1993). Several studies have shown that systems with G0values independent of frequency also show yield stresses in steady shear ﬂow (Lobe and White1979; Davis1971a,b; Ahuja1980). Onogi et al. (1973) was the ﬁrst to propose a correlation between the plateau modulus and the yield stress. They analyzed data on a crosslinked polystyrene latex
dispersed in a polystyrene solution. While depletion ﬂoc-culation was initially described by Asakura and Oosawa (1958), it was not until Heath and Tadros (1983) that the depletion effect was connected to gelation and the rheolog-ical measurements of the modulus. Onogi obtained the yield stress by ﬁtting the non-linearity in their viscosity data with a Casson model, even though their data showed no actual yield point. They obtained G0and G00 as functions of fre-quency, and the data did not display a frequency-indepen-dent plateau. They then proposed a relationship between the yield value and the complex stress deﬁned by
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðG0Þ2þ ðG00Þ2
where G0 is the complex modulus. Gandhi and Salovey (1988) also reported for their carbon black polymer melt systems that the ratio G0=sy was independent of the par-ticle concentration and surface area, but was dependent on the molecular properties of the polymer medium; they found
=sy’10 for a low molecular weight polystyrene sus-pension. Yang et al. (1986) plotted the elastic modulus componentG00c0 versusc0; the maximum of the curve cor-responded to the yield stress measured in steady ﬂow. Franck (1988) reported excellent agreement between the yield stress and the component, G00c0c, where c0c is the critical strain amplitude corresponding to the onset of nonlinear vis-coelastic behavior.
Based on the power law relationship between the yield stress and complex modulus, the following equation is proposed, which is a modiﬁed version of the equation pro-posed by Onogi et al. (1973):
sy¼a G0 b
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðG0Þ2þ ðG00Þ2 q b
For the measured results from all mixtures, the relation-ship between the yield stress and storage shear modulus was
examined. As shown in Fig.6, the mixtures tested in this study showed a good ﬁt to this equation. The variables of the proposed equation were a=2.01, b =0.384, and the coefﬁcient of determination was R2=0.915. The ﬁnal approximation in Eq. (5) provided a similar ﬁt, reﬂecting the relatively small magnitude of G00. The prefactor, a, in Eq. (5), is an order of magnitude larger than the critical strain. Moreover, the dynamic oscillatory measurements are much faster to perform than the shear history that needs to be imposed to obtain the yield stress. Therefore, the measured parameters from the oscillatory shear measurement were utilized to understand the rheological properties. In addition, the viscoelastic properties, which provide information on the microstructure of the sheared suspension should be exam-ined carefully to predict the ﬂow behaviors in a pipe
To understand the ﬂow behavior in a pipe under high pressure, the properties of the lubrication layer between bulk concrete and a pipe wall should be examined. In this study, along with steady shear measurements, oscillatory shear measurements were performed to examine the viscoelastic properties. The following conclusions were obtained:
(1) Due to the migration and redistribution of particles in a pipe under shear by the pumped pressure, the lubrica-tion layer could be considered as being similar to the constitutive cement paste in concrete pumping. (2) To extend the knowledge of the properties of the
lubrication layer, the dynamic oscillatory shear, which is a rheological technique that provides information on viscoelastic materials that are related to the microstruc-tural behavior of ﬂocculated suspension, was mea-sured, which is a relatively new approach to evaluate the rheological performance of pumped concrete. Each of the three mixture systems incorporating BSF, FA, and SF displayed different interactions depending on the types and replacement ratios of the mineral admixtures. Through integrating the results from the steady shear and the dynamic oscillatory measurements it was possible to draw conclusions about the types of interactions occurring.
(3) The yield stress and storage modulus, which arise from fundamental microstructural aspects of the ﬂocculated suspension, can be correlated for all the mixtures tested. The best correlation between the measured yield stress and the complex modulus followed a power law that is somewhat different in form from the mechanical models that are generally used to relate the yield stress to the modulus.
(4) The yield stress is directly related to the ﬂow behaviors in a pipe, which determines the unshared zone in the bulk and governs the microstructure of the sheared suspension. The initial behavior of pumped concrete can be analyzed systematically by examining the viscoelastic properties via oscillatory measurements. Fig. 6 Correlation between yield stresssyand storage shear
This study was supported by the Dongguk University Research Fund of 2015.
This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http:// creativecommons.org/licenses/by/4.0/), which permits unre-stricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
Ahuja, S. K. (1980). Effect of carbon black on the rheological properties of styrene n-butyl methacrylate copolymer melt. In G. Astarita, G. Marrucci, & L. Nicolais (Eds.),Rheology (2nd ed., pp. 469–476). New York, NY: Springer. Aleekseev, S. N. (1952). On the calculation of resistance in the
pipes of concrete pumps.MekhanizatsiyaStroitel’stva, 9(1), 8–13.
Asakura, S., & Oosawa, F. (1958). Interaction between particles suspended in solutions of macromolecules. Journal of Polymer Science, 33, 183–192.
Atzeni, C., Massidda, L., & Sanna, U. (1985). Comparision between rheological models for portland cement pastes. Cement and Concrete Research, 15, 511–519.
Banﬁll, P. F. G., Kitching, D. R. (1990) Use of a Controlled Stress Rheometer to Study the Yield Stress of Oilwell Cement Slurries. In International Conference on Rheology of Fresh Cement and Concrete, University of Liverpool, March 27–29.
Browne, R., & Bamforth, P. (1977). Tests to establish concrete pumpability.Proceedings ACI Journal, 74(5), 193–203. Choi, M. S., Kim, Y. J., & Kwon, S. H. (2013a). Prediction on
pipe ﬂow of pumped concrete based on shear-induced particle migration.Cement and Concrete Research, 52(10), 216–224.
Choi, M. S., Roussel, N., Kim, Y. J., & Kim, J. K. (2013b). Lubrication layer properties during concrete pumping. Cement and Concrete Research, 45(3), 69–78.
Chow, T. W., McIntire, L. V., Kunze, K. R., & Cooke, C. E. (1988). The rheological properties of cement slurries: Effects of vibration, hydration conditions, and additives. SPE Production Engineering, 3, 543–550.
Cooke, C. E., Gonzalez, O. J., & Broussard, D. J. (1988). Pri-mary cementing improvement by casing vibration during cement curing time. SPE Production Engineering, 3, 339–345.
Davis, S. S. (1971a). Viscoelastic properties of pharmaceutical semisolids III: Nondestructive oscillatory testing. Journal of Pharmaceutical Sciences, 60, 1351–1355.
Davis, S. S. (1971b). Viscoelastic properties of pharmaceutical semisolids IV: Destructive oscillatory testing. Journal of Pharmaceutical Sciences, 60, 1356–1365.
Ferry, J. D. (1970). Viscoelastic properties of polymers (2nd ed.). New York: Wiley.
Feys, R., & Schutter, G. D. (2005).Pipe ﬂow velocity proﬁles of complex suspensions, like concrete. Gent, Belgium: Gent University.
Figura, B. D., & Prud’homme, R. K. (2010). Hydrating cement pastes: Novel rheological measurement techniques of the acceleration of gelation.Journal of Rheology, 54, 1363–1378. Franck, A. J. P. (1988). Rheological characterization of sus-pensions-comparison of steady and dynamic techniques. Uhlherr, 2, 327–329.
Gandhi, K., & Salovey, R. (1988). Dynamic mechanical behavior of polymers containing carbon black. Polymer Engineering & Science, 28, 877–887.
Grzeszczyk, S., & Kucharska, L. (1988). The inﬂuence of alkalis on rheological properties of fresh cement pastes. Cement and Concrete Research, 18, 1–8.
Heath, D., & Tadros, T. F. (1983). Rheological investigations of the effect of addition of free polymer to concentrated sterically stabilised polystyrene latex dispersions.Faraday Discussions of the Chemical Society, 76, 203–218. Ingber, M. S., Graham, A. L., Mondy, L. A., & Fang, Z. (2009).
An improved constitutive model for concentrated suspen-sions accounting for shear-induced particle migration rate dependence on particle radius.Int. J. Multiphase Flow, 35, 270–276.
Jacobsen, S., Haugan, L., Hammer, T. A., & Kalogiannidis, E. (2009). Flow conditions of fresh mortar and concrete in different pipes. Cement and Concrete Research, 39(1), 997–1006.
Kaplan, D., Larrard, F. D., & Sedran, T. (2005). Design of concrete pumping circuit. ACI Materials Journal, 102(2), 110–117.
Keating, J., Hannant, D.J. (1990) The use of shear vane to measure the gel strength and dynamic yield strength of oil well cement slurries at high temperature and pressure. International Conference on Rheology of Fresh Cement and Concrete, University of Liverpool, March 27–29.
Lobe, V. M., & White, J. L. (1979). An experimental study of the inﬂuence of carbon black on the rheological properties of a polystyrene melt.Polymer Engineering & Science, 19, 617–624.
Lu, G., Wang, K., & Rudolphi, T. J. (2008). Modeling rheo-logical behavior of highly ﬂowable mortar using concepts of particle and ﬂuid mechanics. Cement and Concrete Composite, 30, 1–12.
Marin, G. (1988). Oscillatory rheometry. In A. A. Collyer & D. W. Clegg (Eds.),Rheological Measurement(pp. 297–343). London, UK: Elsevier.
Morinaga, S. (1973). Pumpability of concrete and pumping pressure in pipe line.Proceeding of a RILEM Seminar Held in Leeds, 3, 1–39.
Onogi, S., Matsumoto, T., & Warashina, Y. (1973). Rheological properties of dispersions of spherical particles in polymer solutions.Transactions. Society of Rheology, 17, 175–190. Papo, A. (1988). The thixotropic behavior of white portland cement pastes. Cement and Concrete Research, 18, 595–603.
Phillips, R. J., Armstrong, R. C., & Brown, R. A. (1992). A constitutive equation for concentrated suspensions that accounts for shear-induced particle migration. Physics of Fluids, 4, 30–40.
Rossig, M., & Frischbeton, F. V. (1974). Insbesondere von Leichtbeton, durch Rohrleitungen, 132, Dr.diss, RWTH. Opladen: Westdeutscher Verlag.
Saaka, A. W., Jenningsa, H. M., & Shah, S. P. (2001). The inﬂuence of wall slip on yield stress and viscoelastic measurements of cement paste. Cement and Concrete Research, 31, 205–212.
Sakuta, M., Yamane, S., Kasami, H., & Sakamoto, A. (1979). Pumpability and rheological properties of fresh concrete.
Proceeding of Conference on Quality Control of Concrete Structures, 2, 125–132.
Schultz, M. A., & Struble, L. J. (1993). Use of oscillatory shear to study ﬂow behavior of fresh cement paste.Cement and Concrete Research, 23, 273–282.
Tattersall, G. H., & Banﬁll, E. E. G. (1983).The rheology of fresh concrete. London, UK: Pitman.
Vassiliev, V. (1953). Flow regime in a concrete pipe.Edition, 7, 42–44.
Weber, R. (1968).The transport of concrete by pipeline. Lon-don, UK: Cement and Concrete Association.
Xuequan, W., & Roy, D. M. (1984). Slag cement utilization: Rheological properties and related characterization.Cement and Concrete Research, 14, 521–528.